Download presentation

Presentation is loading. Please wait.

Published byJonathan Peet Modified over 3 years ago

1
**ELECTRONIC STRUCTURE OF STRONGLY CORRELATED SYSTEMS**

G.A.SAWATZKY UBC PHYSICS & ASTRONOMY AND CHEMISTRY Max Planck/UBC center for Quantum Materials

2
**Some Historical Landmarks**

Bloch Wilson theory of solids 1937 De Boer and Verwey ( NiO-CoO breakdown of band theory 1937 Peierls 3d electrons avoid each other ( basically the Hubbard model) 1949 Mott Metal insulator transition 1950 Jonker, van Zanten, Zener - Pervoskites double exchange 1957 BCS theory of superconductivity 1958 Friedel Magnetic impurities in metals 1959 Anderson superexchange (U>>W) 1962 Anderson model for magnetic impurities in metals 1964 Kondo theory of Kondo effect 1964 Hubbard model- Hohenberg Kohn DFT- Goodenough Transition metal compounds

3
**Some historical landmarks**

1964 Hohenberg Kohn density functional theory and Kohn Sham application to band theory 1964 Goodenough basic principles of transition metal compounds 1965 Goodenough Kanamori Anderson rules for superexchange interactions 1968 Lieb and Wu exact solution of 1D Hubbard model 1972 Kugel Khomskii theory of orbital ordering 1985 Van Klitzing quantum Hall effect 1985 ZSA classification scheme of transition metal compounds 1986 Bednorz and Muller High Tc superconductors 1988 Grunberg and Fert giant magneto resistance

4
It’s the outermost valence electron states that determine the properties Both the occupied and unoccupied ones

5
**Two extremes for atomic valence states in solids**

Where is the interesting physics? Coexistance-----Hybridization Kondo, Mixed valent, Valence fluctuation, local moments, Semicond.-metal transitions, Heavy Fermions, High Tc’s, Colossal magneto resistance, Spin tronics, orbitronics

6
**Extreme valence orbitals**

Recall that the effective periodic corrugation of the potential due to the nuclei screened by the “core” electrons is very small for R>>D leading to free electron like or nearly free electron like behavior. For R<<D the wave functions are atomic like and feel the full corrugation of the screened nuclear potentials leading to quantum tunneling describing the motion of tight binding like models. ATOMIC PHYSICS IS VERY IMPORTANT

7
**Characteristics of solids with 2 extreme valence orbitals**

R>> D R<<D electrons lose atomic identity Form broad bands Small electron electron interactions Low energy scale –charge fluctuations Non or weakly magnetic Examples Al, Mg, Zn, Si Valence Electrons remain atomic Narrow bands Large electron electron interactions (on site) Low energy scale-spin fluctuations Magnetic (Hunds’ rule) Gd, CuO, SmCo3 Many solids have coexisting R>>D and R<<D valence orbitals i.e. rare earth 4f and 5d, CuO Cu 3d and O 2p, Heavy Fermions, Kondo, High Tc,s , met-insul. transitions

8
**Strongly correlated materials**

Often 3d transition metal compounds Often Rare earth metals and compounds Some 4d, 5d and some actinides Some organic molecular systems C60, TCNQ salts Low density 2D electron gases Quantum and fractional quantum Hall effect Strong magnetism is often a sign of correlation

9
**Wide diversity of properties**

Take for example only the transition metal oxides Metals: CrO2, Fe3O4 T>120K Insulators: Cr2O3, SrTiO3,CoO Semiconductors: Cu2O Semiconductor –metal: VO2,V2O3, Ti4O7 Superconductors: La(Sr)2CuO4, LiTiO4, LaFeAsO Piezo and Ferroelectric: BaTiO3 Multiferroics Catalysts: Fe,Co,Ni Oxides Ferro and Ferri magnets: CrO2, gammaFe2O3 Antiferromagnets: alfa Fe2O3, MnO,NiO --- Properties depend on composition and structure in great detail

11
**Phase Diagram of La1-xCaxMnO3**

Uehara, Kim and Cheong R: Rombohedral O: Orthorhombic (Jahn-Teller distorted) O*: Orthorhombic (Octahedron rotated) CAP = canted antiferromagnet FI = Ferromagnetic Insulator CO = charge ordered insulator FM= Ferromagnetic metal AF= Antiferromagnet

12
**High Tc superconductor phase diagram**

13
**Ordering in strongly correlated systems**

Stripes in Nd-LSCO rivers of Charge— Antiferro/ Antiphase DQ < 0.5 e Quadrupole moment ordering Charge inhomogeneity in Bi2212 Pan, Nature, 413, 282 (2001); Hoffman, Science, 295, 466 (2002) DQ ~ 0.1 e DQC ~ 1 e DQO ~ 0

14
**Mn4+ , d3, S=3/2 ,No quadrupole ; Mn3+, S=2, orbital degeneracy**

Mizokawa et al PRB 63, Mn4+ , d3, S=3/2 ,No quadrupole ; Mn3+, S=2, orbital degeneracy

15
**Simplest model single band Hubbard**

Row of H atoms 1s orbitals only Largest coulomb Interaction is on site U The hole can freely Propagate leading to A width The electron can freely Propagate leading to a width E gap = 12.9eV-W The actual motion of the Particles will turn out to be more complicated

16
**For large U>>W One electron per site ----Insulator**

Low energy scale physics contains no charge fluctuations Spin fluctuations determine the low energy scale properties Can we project out the high energy scale? Heisenberg Spin Hamiltonian

17
**Spectral weight transfer**

The real signature of strong correlation effects

18
**Doping a Mott – Hubbard system**

PES EF PES (1-x)/2x N-1 N+1 N-1 2 2 EF EF Meinders et al, PRB 48, 3916 (1993)

19
**In single particle mean field theory states move with doping since the **

average coulomb interaction changes. In correlated electron systems states stay Fixed but spectral weight gets transferred x=0.0 x=0.1 x=0.2 x=0.3 x=0.4 x=0.5 x=0.6 x=0.7 x=0.8 These states would be visible in a two particle addition spectral function x=0.9 Meinders et al, PRB 48, 3916 (1993)

20
**Why are 3d and 4f orbitals special**

Lowest principle q.n. for that l value Large centrifugal barrier l=2,3 Small radial extent, no radial nodes orthogonal to all other core orbitals via angular nodes High kinetic energy ( angular nodes) Relativistic effects Look like core orb. But have high energy and form open shells like valence orb.

21
**A bit more about why 3d and 4f are special as valence orbitals**

Hydrogenic orbital energy non relativistic Relativistic contribution 3d of Cu; binding energy of 3s=120 eV, 3p=70 eV, 3d=10 eV. Strong energy dependence on l due to relativistic effects.

22
**Charge density of outer orbitals of the Rare earths**

Highly confined orbitals will have a large U Charge density of outer orbitals of the Rare earths Atomic radius in solids Elemental electronic configuration of rare earths A rare earth metal For N<14 open shel 5d6s form a broad conduction Band Hubbard for 4f Hubbard U 4f is not full and not empty

23
**Band Structure approach vs atomic**

Delocalized Bloch states Fill up states with electrons starting from the lowest energy No correlation in the wave function describing the system of many electrons Atomic physics is there only on a mean field like level Single Slater determinant states Local atomic coulomb and exchange integrals are central Hunds rules for the Ground state -Maximize total spin-Maximize total angular momentum-total angular momentum J =L-S<1/2 filled shell , J=L+S for >1/2 filled shell Mostly magnetic ground states

24
**DFT and band theory of solids**

The many electron wave function is assumed to be a single Slater determinant of one electron Bloch states commensurate with the periodic symmetry of the atoms in the lattice and so has no correlation in it The single particle wave functions φ contain the other quantum numbers like atomic nlm and spin. k represents the momentum vector The effects of correlation are only in the effective one particle Hamiltonian. NO CORRELATION IN THE WAVE FUNCTION

25
**Configuration interaction approach**

The one electron wave functions in ψ atomic do not possess the symmetry of the lattice which in chemistry is called a broken symmetry ansatz. To include intersite hoping perturbatively we consider mixing in electron configurations with now empty sites and others with two electrons on a site. t t=nn hoping integral Energy =U Mixing in of this excited state wave function amplitude = t/U But there are an infinite Number of these virtual excitations in a configuration interaction approach.

26
**General band theory result for R<<d together with R>>d states**

For open shell bands R<<d R<<d so bands are narrow open thereforE must be at Ef

27
**What do we mean by the states below and above the chemical potential**

The eigenstates of the system with one electron removed or one electron added respectively i.e Photoelectron and inverse photoelectron spectroscopy IPES N+1 N-1

28
**Photoelectron spectroscopy of the rare earths**

29
**Photo and inverse Photo electron spectra of the rare earth **

Metals (Lang and Baer (1984)). 0 is EFermi Solid vertical lines are atomic multiplet theory U

30
**Angular resolved photoelectron spectroscopy (ARPES) of Cu metal **

Thiry et al 1979 ARPES Cu Points –exp. Lines - DFT Cu is d10 so one d hole Has no other d holes to Correlate with so 1 part. Theory works FOR N-1 if the only Important interaction isthe d-d interaction. 3d bands 4s,4p,band

31
We note that for Cu metal with a full 3d band in the ground state one particle theory works well to describe the one electron removal spectrum as in photoelectron spectroscopy this is because a single d hole has no other d holes to correlated with. So even if the on site d-d coulomb repulsion is very large there is no phase space for correlation. The strength of the d-d coulomb interaction is evident if we look at the Auger spectrum which probes the states of the system if two electrons are removed from the same atom If the d band had not been full as in Ni metal we would have noticed the effect of d-d coulomb interaction already in the photoemission spectrum as we will see.

32
**What if we remove 2- d electrons locally**

What if we remove 2- d electrons locally? Two hole state with Auger spectroscopy Auger electron Photoelectron Photon 3d Example is for Cu with A fully occupied 3d band 2p 932eV E(photon)-E(photoelectr) = E(2p) , E (2-d holes)= E(2p)-E(3d)-E(Auger) U = E( 2-d holes) -2xE(1-d hole)

33
**Auger spectroscopy of Cu metal Atomic multiplets Looks like gas phase **

U>W Two hole bound states Hund’s rule Triplet F is Lowest The L3M45M45 Auger spectrum of Cu metal i.e final state has 2 -3d holes on the Atom that started with a 2p hole. Solid line is the experiment. Dashed line is one Electron DFT theory, vertical bars and lables are the free atom multiplets for 8- 3d electrons on a Cu atom . Ef designates the postion of the Fermi level in the DFT . Antonides et al 1977 Sawatzky theory 1977

34
Removal from d9 states Will be U higher in energy Taken from Falicov 1987

35
**Regarding simple models**

Like sinple band Hubbard Sometimes we get so involved in the beauty and complexity of the model that we forget what the validating conditions were and use them outside of the range of validity

36
Closer to real systems We use mainly 3d transition metal compounds as examples More than only spin and charge play a role here Orbital degrees of freedom in partly occupied d orbitals interact with spin and charge degrees of freedom We have to deal with multi band systems

37
**Interplay between spin, charge, lattice and orbital degrees of freedom**

In the large U limit where polarity fluctuations are strongly suppressed in the low energy scale physics THE PHYSICS OF ATOMS AND IONS IN LOWER THAN SPHERICAL SYMMETRY PLAYS AN IMPORTANT ROLE We now deal with crystal and ligand field splittings, Hund’s rule coupling , spin orbit coupling, superexchange interactions, and the role of orbital degeneracy

38
**Some typical coordinations of TM ions**

Octahedral coordination Red=TM ion White =Anion like O2- Tetrahedral coordination Red = TM White =anion like O2- As in NiO As in LiFeAs

39
**Free atom d wave function**

For d states l=-2; m=-2,-1,0,1,2; and for 3d n=3 With spin orbit coupling j=l+s or j=l-s s=spin =1/2 Spin Orbit λ~ meV for 3d and about 3 times larger for 4d For 3d’s the orbital angular momentum is often quenched because λ<< crystal field. THIS IS NOT THE CASE FOR ORBITALLY DEGENERATE T2g states here spin orbit is always important

40
**Real d orbitals in Octahedral coordination**

eg’s have lobes pointing to anion forming sigma bonds and the t2g’s have lobes pointing between the anions with pi bonds

41
**Two kinds of d orbitals generally used**

All have 0 z component Of angular momentum In cubic symmetry the two eg’s and 3 t2gs are 2 and 3 fold degenerate respectively. The spin orbit coupling does not mix the eg orbitals to first order but it does mix the t2g’s which then get split into a doublet and a singlet in cubic symmetry

42
**Crystal and ligand field splitting**

Many of the interesting transition metal compounds are quite ionic in nature consisting of negative anions like O (formally2-) and positive TM ions. Part of the cohesive energy is due to Madelung potentials produced by such an ionic lattice. Recall that O2- is closed shell with 6 2p electrons quite strongly bound to the O . Expanding the potential produced by surrounding ions close to a central TM ion produced a different potential for the eg and t2g orbitals resulting in an energy splitting. The point charge contribution is: The resulting energy shift of the d orbitals is; In first order perturbation theory and the di are the eg and t2g wave functions defined above. Only terms with m=0,4 and n=4 will contribute In cubic symmetry this splits the eg and t2g states by typically 0.5 to 1 eV with in Octahedral coordination the t2g energy lower than the eg energy

43
**There is another larger contribution from covalency or the virtual **

hoping between the O 2p orbitals and the TM d orbitals. Since the eg orbitals are directed to O these hoping integrals will be larger than those for the t2g orbitals eg t2g TM 3d Δ O2p Often about 1-2eV In Oxides Density functional band theory provides good reliable values for the total crystal and Ligand field splitting even though the band structure may be incorrect.

44
**Note the rather broad Cl 2p bands**

And the very narrow Ni 3d bands Split into eg and t2g . Note also the Crystal field spliting of about 1.5eV. Note also that DFT (LDA) predicts a metal for NiCl2 while it is a pale yellow magnetic insulator. Note also the large gap between Cl 2p band and the Ni 4s,4p bands With the 3d’s in the gap. This is a typical case for TM compounds

45
Two new complications d(n) multiplets determined by Slater atomic integrals or Racah parameters A,B,C for d electrons. These determine Hund’s rules and magnetic moments d-O(2p) hybridization ( d-p hoping int.) and the O(2p)-O(2p) hoping ( O 2p band width) determine crystal field splitting, superexchange , super transferred hyperfine fields etc.

46
**Where n,n’ m,m’ are all different. The monopole like coulomb integrals **

The d-d coulomb interaction terms contain density -density like integrals, spin dependent exchange integrals and off diagonal coulomb integrals i.e. Where n,n’ m,m’ are all different. The monopole like coulomb integrals determine the average coulomb interaction between d electrons and basically are what we often call the Hubbard U. This monopole integral is strongly reduced In polarizable surroundings as we discussed above. Other integrals contribute to the multiplet structure dependent on exactly which orbitals and spin states are occupied. There are three relevant coulomb integrals called the Slater integrals; = monopole integral = dipole like integral = quadrupole integral For TM compounds one often uses Racah Parameters A,B,C with ; Where in another convention ; The B and C Racah parameters are close to the free ion values and can be carried over From tabulated gas phase spectroscopy data. “ Moores tables” They are hardly reduced in A polarizable medium since they do not involve changing the number of electrons on an ion.

47
**Reduction of coulomb and exchange in solids**

Recall that U or F0 is strongly reduced in the solid. This is the monopole coulomb integral describing the reduction of interaction of two charges on the same atom However the other integrals F2 andF4 and G’s do not involve changes of charge but simply changes of the orbital occupations of the electrons so these are not or hardly reduced in solids . The surroundings does not care much if locally the spin is 1 or zero. This makes the multiplet structure all the more important!!!!! It can in fact exceed U itself

48
Ballhausen

49
**Multiplet structure for free TM atoms rare **

Earths can be found in the reference VanderMarel etal PRB 37 , (1988)

50
**VanderMarel etal PRB 37 , 10674 (1988)**

51
**Hunds’ rules First the Physics**

Maximize the total spin—spin parallel electrons must be in different spatial orbitals i.e. m values (Pauli) which reduces the Coulomb repulsion 2nd Rule then maximize the total orbital angular momentum L. This involves large m quantum numbers and lots of angular lobes and therefore electrons can avoid each other and lower Coulomb repulsion

52
Hunds’ third rule < half filled shell J=L-S > half filled shell J=L+S Result of spin orbit coupling Spin orbit results in magnetic anisotropy, g factors different from 2, orbital contribution to the magnetic moment, ---

53
**A little more formal from Slater “ Quantum theory of Atomic structure chapter 13 and appendix 20**

One electron wave function We need to calculate Where I,j,r,t label the quantum Numbers of the occupied states and we sum over all the occupied states in the total wave function

57
**Nultiplet structure of 3d TM free atoms**

VanderMarel etal PRB 37 , (1988) Note the high energy scale Note also the lowest energy state for each case i.e. Hunds’ Rule;

58
**Simplified picture of Crystal fields and multiplets**

Determine energy levels assuming only crystal and ligand fields and Hunds’ first rule i.e. Neglect other contributions like C in our former slides and the SO coupling This is a good starting point to generate a basic understanding . For more exact treatments use Tanabe-Sugano diagrams

59
**Crystal fields, multiplets, and Hunds rule for cubic (octahedral) point group**

Free ion Cubic Oh eg (4)J is the energy to flip One of spins around 10DQ= crystal field 10DQ t2g d5; Mn2+, Fe3+ 4J eg S=5/2 No degeneracy t2g t2g d4; Mn3+, Cr2+ 3J eg S=2 two fold degenerate t2g

60
**S=2; 3 fold degenerate d6; Fe2+, Co3+ d2; Ti2+, V3+ S=1; 3 fold**

10DQ t2g d6; Fe2+, Co3+ 3J eg t2g J d2; Ti2+, V3+ S=1; 3 fold degenerate

61
**Physical picture for high spin to low spin transition**

eg 10DQ E(HS)=-10J-4DQ E(LS)= -6J-24DQ HS to LS for 10DQ>2J t2g d6; Fe2+, Co3+ 3J eg t2g eg 10DQ E(HS)=-10J E(LS)=-4J-20DQ HS to LS for 10DQ>3J t2g d5; Fe3+, Co4+ 4J eg 0J t2g

62
**Goodenough Kanamori Anderson rules **

i.e. interatomic superexchange interactions And magnetic structure For example Cu2+---O----Cu2+ as in La2CuO4 and superconductors Cu2+ is d9 i.e. 1 eg hole (degenerate in OH) but split in D4H as in a Strong tetragonal distortion for La2CuO4 structure. The unpaired electron or hole is in a dx2-y2 orbital with lobes pointing to the 4 Nearest O neighbors. Anderson 1961 If the charge transfer energy Δ gets small we have to Modify the superexchange theory New term The sum leads to a huge antiferro Interatomic J(sup) =140meV for the Cuprates

63
**Superexchange for a 90 degree bond angle**

The hoping as in the fig leaves two holes in the intervening O 2p states i.e. a p4 configuration. The lowest energy state According to Hund’s rule is Spin 1. So this process favours A ferromagnetic coupling between the Cu spins. So the net exchange as a function of the bond angle is:

64
**Superexchange between singly occupied t2g orbitals**

dxz z dxz pz x If we now rotate one of the bonds around the z axis the superexchange does not change , but for rotation around the y axis it changes as for eg orbitals. Since

65
**If we have “spectator spins “ as in Mn3+ in OH**

d4; Mn3+, Cr2+ For ferro orbital ordering we will get a strong antiferromagnetic super exchange since the same intervening O 2p orbital is used in intermediate States as in the example above t2g 3J eg t2g For antiferro orbital ordering The factor of 3 in the Hunds’ Rule of Mn is from the “spectator” spins

66
For example in LaMnO3 and the “Colossal” magneto resistance materials La(1-x)CaxMnO3 and now with “orbital ordering “ the extra eg spin has a strong anti- ferro superexchange coupling for ferro orbital ordering i.e. as in the example above for 180 degree bond. But the superexchange is weakly ferromagnetic for antiferro orbital ordering since then both ferro and antiferro terms compete differing only by the Hunds’ rule which now also involves the “spectator “ spins in t2g orbitals. We have neglect the superexchange involving the t2g orbitals here.

67
Zener Double exchange This is important in for example in La(1-x)CaxMnO3 which are colossal magneto resistance materials. Here the extra eg electron pictured in former slides is free to move even if U is large because of the mixed valent nature of the Mn. Some of the Mn3+ (d4) is now Mn3+(d3) which has empty eg orbitals. However the eg electron can only move freely if the spectator t2g spins are ferromagnetically aligned yield a large band width and so a lowering of the kinetic energy. The ferromagnetic exchange is proportional to the one electron band width

68
Orbital degeneracy If there is orbital degeneracy the Jahn Teller theorem tells us that it will be lifted in on way or another at low temperatures. This is because the system can always lower its energy by lifting this degeneracy We distinguish to types those involving eg or t2g orbitals. We consider cubic and OH symmetry to start with Strong Jahn teller ions Weak Jahn Teller ions Strong for strong eg hybridization with ligand and weak for weak t2g hybridization with ligands

69
**How can we lift the degeneracy**

Spin orbit coupling if we have t2g degeneracy. Recall the eg’s do not split with SO. Jahn Teller distortion i.e. from Cubic to tetragonal would split the eg orbitals into d(3z2-r2) and d(x2-y2) (Examples are cuprates Orbital ordering which may be driven by other than electron phonon coupling Charge disproportionation i.e. Where both final configurations are not orbitally degenerate. We will see later why this could happen inspite of a large U

70
**Lattice distortions i.e. the Jahn Teller effect**

Operates via electron phonon coupling with asymmetric phonon modes which locally distort the lattice. For z axis long the doublet would be lowest This lifts the orbital degeneracy for this case Tetragonal Z axis shorter Free ion Cubic Oh eg t2g 3J d(3z2-r2) eg d(x2-y2) dxz,dyz t2g dxy

71
Orbital ordering Consider again the case of Mn3+ with the doubly orbital degenerate eg level in cubic symmetry occupied by only one electron as above. It would be logical in a perovskite structure that long bond axis would alternate say along x and y for two Mn ions sandwiching an O anion as in the next slide

72
For LaMnO3 resonant x ray diffractions yields the orbital occupation structure below with Alternating occupied eg orbitals rotated by 90 degrees as see in the basal plain. The small red arrows indicate the Oxygen displacement resulting from this leading to a so called cooperative Jahn Teller distortion Murakami et al The 300 reflection Is generally forbidden but visible at resonance Because of the orbital ordering See two transitions. One at high Temp for the orbital ordering and one at low T for antiferromagnetic order. The spin ordering in plane is ferromagentic as we would have predicted

73
**Hamiltonian for orbital and spin order (Kugel Khomskii 1982)**

The first term describes spin structure and magnon excitations Second term the Orbital order and Orbiton or d-d exciton excitation Third term is the strong interaction between Orbitons and spin waves this interaction can lead to new bound or spin polaronic like states. In addition we really should have included the electron phonon interaction which would result in lattice distortions depending on the orbital order and in lattice polaronic like effects coupling with orbitons and magnons. Since all these interactions are of the same order of magnitude the situation is very complicated but also very rich in new physical properties and phenomena

74
Doped holes in cuprate As we hole dope the system the O1s to 2p first peak rises very strongly indicating That the doped holes are mainly on O 2p. C. T. Chen et al. PRL 66, 104 (1991)

75
**Is single band Hubbard justified for Cuprates?**

Zhang Rice PRB 1988 37,3759

76
**Problem with ZR singlets**

The combination of O 2p states is not compatible with a band structure state The wave functions are not orthogonal From ZR PRL 37,3759 Note it goes to infinity at k=0, should we see it at Gamma in ARPES? Luckily i goes to 1 for K= Pi/2,Pi/2 and anywhere along the AF zone boundary where the FIRST doped holes go In band theory O 2p does not mix with Cu dx**2-y**2 at Gamma!!!!! SO HOW TO DO THIS PROPERLY FOR HIGH DOPING?

77
**Is this only a problem for the Cuprates?**

What about the Nickalates, Manganites, Cobaltates etc?

78
**Note the high “pre- Edge feature and the Spectral weight**

Kuiper et al PRL (1989) LixNi1-x O A CHARGE TRANSFER GAP SYSTEM HOLES IN O Note the high “pre- Edge feature and the Spectral weight Transfer from high To low energy scales Just as in the cuprates The holes are mainly on O and not on Ni.!!

79
**Note the huge O 1s -2p prepeak just as in the cuprates HOLES ON O**

LNO thin film on LSAT Sutarto, Wadati, Stemmer UCSB Note the huge O 1s -2p prepeak just as in the cuprates HOLES ON O

80
**Can we renormalize and get rid of the anion states?**

Similar to the Zhang Rice singlets in the cuprates?

81
**Oxides are more complicated**

Remember at surfaces U is increased, Madelung is decreased, W is decreased

82
For divalent cations

83
High oxidation states In general we expect the charge transfer energy to strongly decrease for higher oxidation states This would mean a different starting point i.e. Cu Cu2+L Ni Ni3+L Co Co3+L Fe Fe3+L Mn4+??? The charge degrees of freedom are on Oxygen

84
**Charge disproportionation without moving charge**

Consider ReNiO3 Ni3+ on average but label it as Ni2+L Then each Ni is surrounded by 2 L holes in ReNiO3 ( 1 hole per 3 O) 2Ni3++ Ni Ni4+ Two holes in O2p Orbital in octahedron With central eg symmetry Ni2+ no JT Each second Ni2+ has an octahedron of O with two holes of Eg symmetry in bonding orbital's I.e. d8 L2 No Jahn Teller problem anymore

85
Torrance et al PRB 42, 8209

86
**The nickaltes i.e. RENiO3 Lets associate the two holes (with S=1)**

with one Ni which will then be a S=0 cluster Because of Jpd. The octahedron will contract leaving the other Ni neighbors in a d8 S=1 state. This gives the correct structure at low T and in fact also gives the correct spin structure . Effective disproportionation without moving charge. THIS STATE SEEMS TO BE NEARLY DEGNERATE WITH A METALLIC ITINERANT O HOLE STATE

87
**What do we mean by the conductivity gap in a material**

The minimum energy cost to remove an electron minus the maximum energy gain to add one to the ground state E gap = E0 (N-1) +E0(N+1) – 2E0(N) N is the number of electrons in The ground state. E0 here stands For the lowest energy state in each case.

89
C60

91
**Electronic Structure of oxide surfaces and interfaces A path to new materials and devices?**

92
**Summary Surface electronic structure of Oxides**

Reconstruction at Polar surfaces and interfaces; electronic, ionic, chemical There still is a lot of uncertainty/controversy concerning the electronic structure changes at oxide surfaces and interfaces. We need improved materials and improved methods to study buried interfaces.

96
**New quantum materials Based on Oxides**

Interplay charge, spin, orbital and lattice Interface control : strain- pressure, internal electric fields, local symmetry changes which change crystal fields and superexchange interactions

97
**Correlated Electrons in transition metal compounds**

dn dn dn-1 dn+1 U : Cu (d9) O (p6) Δ : p6 dn p5 dn+1 U = EITM – EATM - Epol Δ = EIO – EATM - Epol + δEM If Δ < (W+w)/2 Self doped metal Epol depends on surroundings!!! EI ionization energy EA electron affinity energy EM Madelung energy J.Hubbard, Proc. Roy. Soc. London A 276, 238 (1963) ZSA, PRL 55, 418 (1985) At a surface the charge transfer energy decreases , And U also increases and the band widths also decrease

98
**Novel Nanoscale Phenomena in Transition-Metal Oxides**

Ionic Oxide Polar Surfaces Stabilization of polar surfaces by epitaxy Correlated Electron System Surfaces Kinks and steps stabilized by epitaxy NiO (100) D Metallic steps Superconducting Copper oxides Applications: Novel SC; QuBits Sr O -1 +2 -2 +1 < 10 ML LaMnO3 eg t2g Mn3+ 3d 4 Strained 2D Layers Positive and negative pressure Applications: CMR; M-I Transition; Orbital Ordering Transparent insulator ½ metallic FM Applications: Spintronics; CMR Electronic Structure of Interfaces Metal-Insulator interface: gap suppression Applications: Molecular Electronics; Fuel Cells; Thermal Barrier Coatings Artificial Molecules Embedded into a Material Ca, Mg, Sr, Ni vacancies or O-N substitution in oxides New class of magnetic materials by ‘‘low-T’’ MBE growth Applications: Spintronics; Novel Magnets J O N

99
**Surface Madelung potential**

Divide the solid into two halves plus a single layer in between . The single layer plus one of the two halves would form a half infinite solid with the single layer as the surface. An ion marked X in the single layer would feel a MP due to the half infinite plus that produced by the single layer. The bulk MP at the same ion X would be twice that of the half infinite solid plus that from the single layer. MP(bulk)=MP(left half)+MP (right half)+MP(single layer)= 2MP(half infinite)+MP(single Layer) MP(half infinite)=1/2 MP(Bulk) –MP(single layer) MP(surface)=MP(half infinite)+ MP(single layer) =1/2(MP(bulk)+MP(single layer)) X

100
**Madelung potentials for rock salt structure TM monoxides**

Two extreme cases are considered ,fully ionic i.e. 2+ and 2- charges and 1+,1- charges

101
**Madelung potential depends on coordination number**

Drawn is a 110 surface where TM has 2 missing O2- Neighbors. The front face is 100 and in it each TM ha one O2- nearest neighbor missing Basically this describes the systematics of the surface Madelung potential Remember that for the charge transfer gap materials the band gaps are determined by the charge transfer energy which changes by twice the change in the Madelung potential or by 2.6 eV for the monovalent case and twice this for the divalent case

102
**Metallic states for negative charge transfer gap energies as could happen at step edges.**

103
**The theory of systems with negative charge transfer gap energies**

This is really complicated since we now cannot use our simple non metallic ansatz. We then have a problem of a high density of local spins in dn states with strong hybridization and exchange with the holes on O. The case I alluded to of LaNiO3 is perhaps such an example. We might be able make interesting new materials using vicinal or Stepped surfaces to generate negative chanrge transfer gaps.

104
**Systemtics of conductivity gaps gaps**

105
**Neutral (110) surfaces of NiO**

Slab of 7 NiO layers LSDA+U: U=8eV J=0.9eV Band gap at surface decreases from 3 eV to 1.2 eV Step edges could be 1D strongly correlated metals Note the splitting of the eg unoccupied bands due To the symmetry lowering at the surface

106
**SrTiO3 (001) surface TiO2 terminated surface PDOS y O 2p Ef Ti 3d Ef x**

The degeneracy of states at the surface is lifted due to reduced symmetry. Surface band gap is reduced by 0.8eV from 1.9eV in the bulk. Reduction of Madelung potential and hybridization at the surface of ionic material.

107
**What happens for surfaces with a net charge and a +,-,+,- alternation of layers?**

These are so called polar surfaces and they have an infinite energy and cannot exist as the termination of a bulk materials. SO WHAT HAPPENS? These are the examples that yield a metallic and also superconducting interface between two insulating materials of which one is polar.

109
**The basic physics involved in the new **

POLAR SURFACES The basic physics involved in the new discoveries of Spectacular properties of some oxide interfaces? LaAlO3/SrTiO3 Interface of two insulators = superconductor Hwang, Mannhart, Trisconne, Blanck,

110
**Classification of Ionic Crystals Surfaces**

SrO TiO2 Type 1 : all planes are charge neutral (001) surface of tetravalent perovskites SrTiO3 ... TiS2 -2 +4 LiFeAs +1/2 -3/2 +2 Type 2 : planes are charged but there is no dipole in repeat unit (001) surface of trivalent perovskites LaAlO3, LaMnO3 ... -1 +1 LaO AlO2 Type 3 : planes are charged and there is dipole in repeat unit P.W. Tasker, J. Phys. C 12, 4977 (1979) Thanks to Ilya Elfimov

111
**What happesn if we have a polar surface?**

Take the NaCl Rock salt structure as in NiO, CaO, MgO, MnO etc Alternating layers of +2 ,-2 charges in the ionic limit.

112
**LSDA Band Structure of CaO (111) Slab terminated with Ca and O**

-10 -5 5 10 Γ K M A L H Energy (eV) -10 -5 5 10 Γ K M A L H Ca 4s Spin Up Spin Down O 2p 12 But surface is metallic! And ferromagnetic!half metallic ferromagnet Note: Bulk material (no surface) is an insulator 10 8 Energy (eV) 6 4 2 -2 -4 L X W L K

113
**Polar Why are polar surfaces i.e. type 3 different?**

Asymmetric boundary condition: Diverging potential Polar E = σ/ε0 E = 0 +Q x +Q x -Q x -Q x Q- V Q+ d σd ε0 2σd (111) Remember Gauss’s Law? The field outside an infinite charged plane of small thickness is given by

114
**Simple explanation : big capacitor**

z V z z V + Q/2 + Q/2 - Q/2 + Q/2 - Q/2 2E E E = + - Q/2 2E * N * d E * d V E * (2N-1)*d Solution to polar catastrophe problem is to get rid of big capacitor.

115
**Potential difference between two surfaces of the slab**

Vacuum +(Q - q) -Q N - number of bilayers d - distance between planes A - unit area Vdiv Vbulk +Q Vslab Vbulk Vdiv 2xVbulk MgO (111), 6BL surf -Q +Q -Q +Q -(Q - q) Vacuum Vdiv MgO (111) 1002eV LaAlO3 (001) 418eV For 18 bilayer thick films the Potential difference is in eV) Far above the Zener breakdown Limit =Egap

116
**Polar surfaces and interfaces**

Cannot be compensated by simply moving things across the interface as in intermixing Cannot be compensated by moving around charges outside of the polar material as for example compensating for LAO at the LAO/STO interface by moving electrons around O vacancies in STO to the interface! We need to add charge of order 1 per unit cell to the region around the interface and an equal an opposite charge at the surface or other interface. The materials remains charge neutral

117
Interesting materials in which electronic reconstruction can strongly alter properties and which can be used for interface engineering to develop new devices with exotic properties. Super Conductors: YBa2Cu3O6+δ (Cu) 1+ (BaO) 0 (CuO2) 2- (Y) 3+ (CuO2 ) 2- Perovskites: LaTMO3 (Ti,V,Mn ...) Spin, charge and orbital ordering (001) surface in trivalent compounds LaOFeAs 1+ 1- Simple oxides: SrO, NiO, MnO ... (110) surface (111) surface

118
**Some key papers on polar surfaces and interfaces**

R. Lacman, Colloq. Int. C.N.R.S. 152 (1965) 195 D. Wolf, Phys. Rev. Lett. 68 (1992) 3315. H.-J. Freund and E. Umbach, Eds., Adsorption on Ordered Surfaces of Ionic Solids and Thin Films, Vol. 33 of Springer Series in Surface Science (Springer, Berlin, 1993). Hesper et al PRB 62, coined the phrase Electronic Reconstruction for K3C60 surfaces Ohtomo and H. Y. Hwang Nature 427, 423 (2004) Insulating Oxide heterostructures

119
**Superconducting interface SrTiO3/LaAlO3**

N.Reyren et al Science express 317, Superconducting interface SrTiO3/LaAlO3

120
**There are several ways to stabilize a polar surface**

Oxygen vacancies at the surface (remove O2- i.e. charge or it won’t work!) Facetting i.e. piramids with 100 faces (again result has to be removing charge!!) Adsorbed molecules i.e. OH- on outermost Mg surface (again OH- replaces O2- as outer layer) Terminating monovalent ions Electronic reconstruction (move charge from one surface to the other)

121
**Types of reconstruction**

Electronic Ionic Chemical +Q +Q/2 +Q -Q -Q -Q +Q/2 +Q +Q +Q -Q -Q/2 -Q -Q Rearrangement of electrons Rearrangement of Ions faceting plus charging Vacancies or add Ions (K+) or OH- adds charge K-depositon: M.A. Hossain et al., Nat. Phys. 4, 527 (2008). NiO(111): D. Cappus et al., Surf. Sci. 337, 268 (1995). K3C60: R. Hesper et al., Phys. Rev. B 62, (2000). NiO(111): D. Cappus et al., Surf. Sci. 337, 268 (1995).

122
**Electronic Reconstruction**

Energetically favourable in ionic systems with small band gaps and in systems with multivalent components ( Ti,V,C60,Ce,Eu ----)

123
**Interfaces involving polar surfaces**

Interfaces between polar and non polar srufaces as In SrTiO3 and LaAlO3 for example can be magnetic And Metallic . They will be “self doped” perhaps even superconducting The best candidates for electronic reconstruction at surfaces and interfaces is if one component does not mind changing its valence ! So use systems exhibiting multi valence or mixed valence behaviour Ti,V, are good examples

124
**Examples of ad atom stabilization of Polar surfaces**

NiO grown by MBE is covered by a monolayer of OH - =1/2 the charge of the Ni2+ layer underneath and therefore stable MnS single crystals grown with vapor transport methods yield large crystals with 111 facets???? Covered by a single layer of I- and the crystal grows underneath. Like a surfactant ½ Ba2+ missing on the surface of BaFe2As2 Elfimov has DFT calculations of O vacancies , and various forms of add atoms K+ ad ions on YBCO

125
**Atomic reconstruction**

Facetting or ion displacements forming dipole moments to compensate for the electric field.

126
**Octopolar reconstruction of MgO (111) slab**

Top view Side view Effective surface layer charge = +2(3/4) -2(1/4) = +1 Note that in or to be totally charge neutral other surfaces must change their charge accordingly by one of 3 methods described. If the other surface is an interface the charge could be in the substrate as proposed for the system LAO/STO

127
Summary Reduced dimensionality enforces correlations and could result in self doping= dramatic change in the properties of materials Thin films of Oxides on highly polarizable substrates can lead to band gap narrowing and changes in exchange interactions Polar surfaces/ interfaces-electronically reconstruct = Metals,ferromagnets, even superconductors Point defects like Cation vaqcancies may result in local magnetic moments being formed due to a molecular Hund’s rule coupling involving O 2p holes leading to ferromagnets.

128
**States I have a core hole on atom i and a valence electron**

This depends on the local electronic structure Enhancement by 3-4 orders of magnitude at resonance.

129
**Experimental Geometry**

2p d transition Cu2+ 3d9 Cu1+ 3d10 q f

130
**Zooming-in on different Cu’s: Tuning Polarization**

E//ac E//ab At L3 edge, Photon energy (eV)

131
**Energy Loss is t2g-eg splitting These form d-d excitons or also **

S=2, 3 fold degenerate d6; Fe2+, Co3+ eg eg t2g t2g 3J eg eg t2g t2g Energy Loss is t2g-eg splitting These form d-d excitons or also called orbitaons

132
**Resonant inelastic x ray scattering**

PRL 105, (2010) SLS Ghiringhelli et al RIXS on Sr2CuO2Cl2 Resonant inelastic x ray scattering d-d excitons Due to crystal fields Magnon dispersion

133
**igure 2: Experimental data.**

Similar presentations

OK

Chapter 7 Atomic Structure & Periodicity. Electromagnetic Radiation O Waves (wavelength, frequency & speed) O c (page 342: #39) O Hertz O Max Planck.

Chapter 7 Atomic Structure & Periodicity. Electromagnetic Radiation O Waves (wavelength, frequency & speed) O c (page 342: #39) O Hertz O Max Planck.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Animated ppt on magnetism video Ppt on review of related literature thesis Ppt on total knee replacement Ppt on simultaneous ac-dc power transmission Knowledge based view ppt online Ppt on maths for class 3 Ppt on digital media broadcasting system Ppt on air pollution in hindi Ppt on indian construction industry Moving message display ppt online